- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Advances in OptoElectronics

Volume 2012 (2012), Article ID 347875, 5 pages

http://dx.doi.org/10.1155/2012/347875

## Conditions of Perfect Imaging in Negative Refraction Materials with Gain

^{1}State Key Laboratory of Optoelectronic Materials and Technologies, Sun Yat-sen University, Guangzhou 510275, China^{2}Department of Physical Electronics, School of Electrical Engineering, Faculty of Engineering, Tel Aviv University, 69978 Tel Aviv, Israel^{3}Chemical Physics Department, Weizmann Institute of Science, 76100 Rehovot, Israel

Received 29 June 2012; Accepted 3 October 2012

Academic Editor: Alexandra E. Boltasseva

Copyright © 2012 Haowen Liang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

Light propagation is analyzed in a negative refraction material (NRM) with gain achieved by pumping. An inherent spatial “walk-off” between the directions of phase propagation and energy transfer is known to exist in lossy NRMs. Here, the analysis is extended to the case where the NRM acts as an active material under various pumping conditions. It is shown that the condition for perfect imaging is only possible for specific wavelengths under special excitation conditions. Under excessive gain, the optical imaging can no longer be perfect.

#### 1. Introduction

Negative refraction is known to offer a wide range of potential applications [1–4]. However, losses, which are an inherent feature of the negative refraction, present a major impediment to the performance of NRMs [5–9]. To overcome these problems, NRMs with gain were proposed to compensate the losses, even to turn the materials into amplified systems. Nevertheless, it is often stated that the gain will destroy the negative refraction due to causality considerations [10], although the statement was disputed by a theory demonstrating that negative refraction may be preserved in a limited spectral region [11, 12].

Common methods to introduce gain in NRMs include optical parametric amplification (OPA) [13] and externally pumped gain materials [14–18]. Optical imaging needs to collect both propagating and evanescent waves. However, only within a limited range may the wave vectors receive gain from OPA because of the strict phase-matching condition, the application of OPA to achieve perfect imaging in NRMs is not possible.

In this paper, we demonstrate that, under the action of the pumping gain, lossless and amplified light propagation may occur in a special spectral window of the NRM. The propagation behavior is shown to be closely related to the dispersion and pumping configuration. Propagation in NRMs is also examined in different pumping configurations.

##### 1.1. Spatial “Walk-Off” in Lossy NRMs

Light incidents from free space onto a homogeneous, isotropic, lossy NRM, of permittivity and permeability , were studied in detail [8]. The complex effective refractive index is then defined as or . In free space, the incident wave vector is real, while in the lossy NRM, the wave vector is complex. At a given optical frequency , this implies that for both the propagating wave () and the evanescent one ().

To analyze light propagation in the NRM, the phase and group velocities are expressed as and , where and are determined by the NRM dispersion. The energy propagation is approximately determined by the group velocity under the assumption of low losses [19–21]. The Poynting vector can also be used to define the energy propagation.

For complex vectors and , the direction of the phase propagation and energy transfer in the wave packet are determined by their real parts [22]:
In an ideal NRM, where the refractive index is negative without losses, the phase velocity and group velocity are strictly antiparallel [1, 19]. However, (1) and (2) show that the group velocity is no longer antiparallel because of the contribution of the last term in (2). This *spatial “walk-off,”* that is, the noncollinearity between the phase propagation and the energy transfer, becomes obvious in a homogenous, isotropic, lossy NRM. The angle between the phase velocity and the group velocity is
with the “walk-off” angle defined as .

The propagation behavior is discussed here for both propagating and evanescent waves. The dispersive curve is described as the Lorentz model, with , , and s^{−1}, s^{−1}, s^{−1} in Figure 1(a) for the real and imaginary parts of the refractive index. For a typical propagating wave with , the size of the “walk-off” is numerically simulated as shown in Figure 1(b). The analysis of the “walk-off” can be extended to evanescent waves with , where it is found that the “walk-off” dramatically increases with , also shown in Figure 1(b).

For perfect focusing, the “walk-off” appearing at different should be suppressed. It was shown that this goal can be achieved by a pumping gain scheme [18]. Here, we show, in a pumped four-level model of signal amplification, that the realization of perfect imaging is possible only for a specific wavelength under strict pumping condition.

#### 2. NRMs with Pumping Gain

Four-level systems represent conventional gain media. The intensity of light in a chosen spectral interval can be amplified in NRMs by introducing an extra term in the electrical field susceptibility [14, 17, 23]. It is assumed here that the gain medium is pumped in the linear regime, and no gain saturation arises. Accordingly, the population of the ground level (which can be considered as the population of the gain medium) is much larger than in the other three levels as per the usual pumping condition. With the definition of polarization , the permittivity, with the extra term in the susceptibility, is given by

As shown below, the last term of (4) is crucial to the performance of the gain-compensated NRMs. The components of the effective refractive index, and , are shown in Figure 2.

Whereas the optical losses in the NRM can be effectively compensated by pumping, as shown in Figure 2(b), an amplification of the input signal is achievable; the elimination of the “walk-off” depends on both the real and imaginary parts of the refractive index. The ideal case is the one with and , giving rise to perfect imaging [1, 6]. However, as shown in Figure 2, this condition holds only at the optimal frequency where s^{−1} under appropriate pumping conditions.

Optical imaging with resolution above or below the diffraction limit depends on the system’s ability to recover the wavevector’s component for either propagating or evanescent waves. Figure 3(b) shows the size of the “walk-off” for different with the appropriate pumping rate of s^{−1}. The propagating waves correspond to , while the evanescent ones correspond to . After introducing the pumping gain, a red shift is observed in the curve. At the optimal frequency ( s^{−1}) where , the angles between the group and phase velocities are strictly antiparallel for all . Because of the antiparallel directions of the energy transfer and phase propagation, the spatial “walk-off” is suppressed, so that the ability of directional transmission (for the propagating waves) and perfect focusing (for evanescent waves in the near-field) will be preserved. Thus, the pumping can effectively cancel the losses only in a limited spectral region, under appropriate pumping conditions. This conclusion is in agreement with those reported in [11, 12].

By contrast, the propagation in an active NRM under excessive pumping exhibits a peculiar behavior. Figure 3(c) shows the “walk-off” angles at different for excessive pumping rate (here s^{−1}) at the frequency where (here s^{−1}). The angles are then larger than 180°, indicating that the “walk-off” reappears, with the respective angles . The “walk-off” becomes more significant at larger . It also shows that increases dramatically with the increase of for the evanescent wave with . Hence, the perfect focus for the near-field component is impossible under excessive pumping. Notice that because of the red shift in , the “walk-off” is suppressed at the frequency of s^{−1}, where (the red arrow in Figure 3(c)). However, perfect lensing requires [1, 6], hence the perfect focus cannot be obtained under excessive pumping.

In order to achieve perfect focusing, the pumping rates should be reduced and the pumping central frequencies should be blue-shifted, as shown in Figure 3(c). Light with all values of can then perfectly focus through the slab.

#### 3. Conclusions

To conclude, we have analyzed the effect of gain on the negative refraction in NRMs. In a lossy NRM, even though it is isotropic and homogeneous, the group and phase velocities are not strictly antiparallel, yielding a spatial “walk-off”, which may restrict the applications of NRMs in a variety of fields. By introducing gain, losses can be effectively reduced, and light amplification can be realized within a narrow spectral range. Appropriately setting the gain to strictly cancel the losses, the “walk-off” for both propagating and evanescent waves can be effectively eliminated for all values of , leading to an ideal NRM. However, for excessively pumped NRMs, the spatial “walk-off” reappears. Thus, the use of optical pumping to realize perfect imaging is restricted to a very narrow spectral region, under precisely defined pumping conditions. An alternative method of overcoming NRM losses without signal distortion may involve self-induced transparency (SIT) solitons, which were predicted in metamaterials [24], in analogy with SIT in other resonantly absorbing structures [25, 26].

#### Acknowledgments

This work is supported by The National Key Basic Research Special Foundation (G2012CB921904) and by the Chinese National Natural Science Foundation (10934011).

#### References

- J. B. Pendry, “Negative refraction makes a perfect lens,”
*Physical Review Letters*, vol. 85, no. 18, pp. 3966–3969, 2000. View at Publisher · View at Google Scholar · View at Scopus - R. A. Shelby, D. R. Smith, and S. Schultz, “Experimental verification of a negative index of refraction,”
*Science*, vol. 292, no. 5514, pp. 77–79, 2001. View at Publisher · View at Google Scholar · View at Scopus - K. L. Tsakmakidis, A. D. Boardman, and O. Hess, “‘Trapped rainbow’ storage of light in metamaterials,”
*Nature*, vol. 450, no. 7168, pp. 397–401, 2007. View at Publisher · View at Google Scholar · View at Scopus - H. G. Chen, C. T. Chan, and P. Sheng, “Transformation optics and metamaterials,”
*Nature Materials*, vol. 9, no. 5, pp. 387–396, 2010. View at Publisher · View at Google Scholar · View at Scopus - R. W. Ziolkowski and E. Heyman, “Wave propagation in media having negative permittivity and permeability,”
*Physical Review E*, vol. 64, no. 5, Article ID 056625, 2001. View at Scopus - D. R. Smith, D. Schurig, M. Rosenbluth, S. Schultz, S. A. Ramakrishna, and J. B. Pendry, “Limitations on subdiffraction imaging with a negative refractive index slab,”
*Applied Physics Letters*, vol. 82, no. 10, pp. 1506–1508, 2003. View at Publisher · View at Google Scholar · View at Scopus - A. G. Ramm, “Does negative refraction make a perfect lens?”
*Physics Letters A*, vol. 372, no. 43, pp. 6518–6520, 2008. View at Publisher · View at Google Scholar · View at Scopus - Y.-J. Jen, A. Lakhtakia, C.-W. Yu, and C.-T. Lin, “Negative refraction in a uniaxial absorbent dielectric material,”
*European Journal of Physics*, vol. 30, no. 6, pp. 1381–1390, 2009. View at Publisher · View at Google Scholar · View at Scopus - W. H. Wee and J. B. Pendry, “Looking beyond the perfect lens,”
*New Journal of Physics*, vol. 12, Article ID 053018, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. I. Stockman, “Criterion for negative refraction with low optical losses from a fundamental principle of causality,”
*Physical Review Letters*, vol. 98, no. 17, Article ID 177404, 2007. View at Publisher · View at Google Scholar · View at Scopus - P. Kinsler and M. W. McCall, “Causality-based criteria for a negative refractive index must be used with care,”
*Physical Review Letters*, vol. 101, no. 16, Article ID 167401, 2008. View at Publisher · View at Google Scholar · View at Scopus - K. J. Webb and L. Thylén, “Perfect-lens-material condition from adjacent absorptive and gain resonances,”
*Optics Letters*, vol. 33, no. 7, pp. 747–749, 2008. View at Publisher · View at Google Scholar · View at Scopus - A. K. Popov and V. M. Shalaev, “Compensating losses in negative-index metamaterials by optical parametric amplification,”
*Optics Letters*, vol. 31, no. 14, pp. 2169–2171, 2006. View at Publisher · View at Google Scholar · View at Scopus - P. P. Orth, J. Evers, and C. H. Keitel, “Lossless negative refraction in an active dense gas of atoms,” 2007, http://arxiv.org/abs/0711.0303.
- A. Fang, T. Koschny, M. Wegener, and C. M. Soukoulis, “Self-consistent calculation of metamaterials with gain,”
*Physical Review B*, vol. 79, no. 24, Article ID 241104, 2009. View at Publisher · View at Google Scholar · View at Scopus - Y. Sivan, S. Xiao, U. K. Chettiar, A. V. Kildishev, and V. M. Shalaev, “Frequency-domain simulations of a negativeindex material with embedded gain,”
*Optics Express*, vol. 17, no. 26, pp. 24060–24074, 2009. View at Publisher · View at Google Scholar · View at Scopus - S. Wuestner, A. Pusch, K. L. Tsakmakidis, J. M. Hamm, and O. Hess, “Overcoming losses with gain in a negative refractive index metamaterial,”
*Physical Review Letters*, vol. 105, no. 12, Article ID 127401, 2010. View at Publisher · View at Google Scholar · View at Scopus - S. Xiao, V. P. Drachev, A. V. Kildishev et al., “Loss-free and active optical negative-index metamaterials,”
*Nature*, vol. 466, no. 7307, pp. 735–738, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. W. McCall, “What is negative refraction?”
*Journal of Modern Optics*, vol. 56, no. 16, pp. 1727–1740, 2009. View at Publisher · View at Google Scholar · View at Scopus - V. Gerasik and M. Stastna, “Complex group velocity and energy transport in absorbing media,”
*Physical Review E*, vol. 81, no. 5, Article ID 056602, 2010. View at Publisher · View at Google Scholar · View at Scopus - L. Muschietti and C. T. Dum, “Real group velocity in a medium with dissipation,”
*Physics of Fluids B*, vol. 5, no. 5, pp. 1383–1397, 1993. View at Scopus - M. Born and E. Wolf,
*Principals of Optics*, Cambridge University Press, 7th edition, 1999. - A. A. Govyadinov, V. A. Podolskiy, and M. A. Noginov, “Active metamaterials: sign of refractive index and gain-assisted dispersion management,”
*Applied Physics Letters*, vol. 91, no. 19, Article ID 191103, 2007. View at Publisher · View at Google Scholar · View at Scopus - J. Zeng, J. Zhou, G. Kurizki, and T. Opatrny, “Backward self-induced transparency in metamaterials,”
*Physical Review A*, vol. 80, no. 6, Article ID 061806, 2009. View at Publisher · View at Google Scholar · View at Scopus - M. Blaauboer, B. A. Malomed, and G. Kurizki, “Spatiotemporally localized multidimensional solitons in self-induced transparency media,”
*Physical Review Letters*, vol. 84, no. 9, pp. 1906–1909, 2000. View at Scopus - T. Opatrný, B. A. Malomed, and G. Kurizki, “Dark and bright solitons in resonantly absorbing gratings,”
*Physical Review E*, vol. 60, no. 5, pp. 6137–6149, 1999. View at Scopus